Durometer is one of several measures of the hardness of a material. Hardness may be defined as a material's resistance to permanent indentation. The durometer scale was defined by Albert F. Shore, who developed a measurement device called a durometer in the 1920s. The term durometer is often used to refer to the measurement, as well as the instrument itself. Durometer is typically used as a measure of hardness in polymers, elastomers, and rubbers.
There are several scales of durometer, used for materials with different properties. The two most common scales, using slightly different measurement systems, are the ASTM D2240 type A and type D scales. The A scale is for softer plastics, while the D scale is for harder ones. However, the ASTM D2240-00 testing standard calls for a total of 12 scales, depending on the intended use; types A, B, C, D, DO, E, M, O, OO, OOO, OOO-S, and R. Each scale results in a value between 0 and 100, with higher values indicating a harder material.
Method of measurement
Durometer, like many other hardness tests, measures the depth of an indentation in the material created by a given force on a standardized presser foot. This depth is dependent on the hardness of the material, its viscoelastic properties, the shape of the presser foot, and the duration of the test. ASTM D2240 durometers allows for a measurement of the initial hardness, or the indentation hardness after a given period of time. The basic test requires applying the force in a consistent manner, without shock, and measuring the hardness (depth of the indentation). If a timed hardness is desired, force is applied for the required time and then read. The material under test should be a minimum of 6.4 mm (.25 inch) thick.
Test setup for type A & D Durometer Indenting foot Applied mass [kg] Resulting force [N] Type A Hardened steel rod 1.1 mm - 1.4 mm diameter, with a truncated 35º cone, 0.79 mm diameter 0.822 8.064 Type D Hardened steel rod 1.1 mm - 1.4 mm diameter, with a 30º conical point, 0.1 mm radius tip 4.550 44.64
The ASTM D2240 standard recognizes twelve different durometer scales using combinations of specific spring forces and indentor configurations. These scales are properly referred to as durometer types; ie a durometer type is specifically designed to determine a specific scale, and the scale does not exist separately from the durometer. The table below provides details for each of these types, with the exception of Type R.
Durometer Type Configuration Diameter Extension Spring force A 35° truncated (frustrum) cone 1.40 mm (0.055 in) 2.54 mm (0.100 in) 822 gf (8.06 N) C 35° truncated (frustrum) cone 1.40 mm (0.055 in) 2.54 mm (0.100 in) 4,536 gf (44.48 N) D 30° cone 1.40 mm (0.055 in) 2.54 mm (0.100 in) 4,536 gf (44.48 N) B 30° cone 1.40 mm (0.055 in) 2.54 mm (0.100 in) 822 gf (8.06 N) M 30° cone 0.79 mm (0.031 in) 1.25 mm (0.049 in) 78 gf (0.76 N) E 2.5 mm (0.098 in) spherical radius 4.50 mm (0.177 in) 2.54 mm (0.100 in) 822 gf (8.06 N) O 1.20 mm (0.047 in) spherical radius 2.40 mm (0.094 in) 2.54 mm (0.100 in) 822 gf (8.06 N) OO 1.20 mm (0.047 in) spherical radius 2.40 mm (0.094 in) 2.54 mm (0.100 in) 113 gf (1.11 N) DO 1.20 mm (0.047 in) spherical radius 2.40 mm (0.094 in) 2.54 mm (0.100 in) 4,536 gf (44.48 N) OOO 0.635 mm (0.0250 in) spherical radius 10.7 mm (0.42 in) - 11.6 mm (0.46 in) 2.54 mm (0.100 in) 113 gf (1.11 N) OOO-S 10.7 mm (0.42 in) radius disk 12.0 mm (0.47 in) 5.0 mm (0.20 in) 197 gf (1.93 N)
Note: "Type R is a designation, rather than a true ‘type’. The R designation specifies a presser foot diameter (hence the R, for radius, obviously D could not be used) of 18 ± 0.5 mm (0.71 ± 0.02 in) in diameter, while the spring forces and indentor configurations remain unchanged. The R designation is applicable to any D2240 Type, with the exception of Type M; the R designation is expressed as Type xR, where x is the D2240 type, eg aR, dR, etc; the R designation also mandates the employment of an operating stand".
The final value of the hardness depends on the depth of the indenter after it has been applied for 15sec on the material. If the indenter penetrates 2.54 mm (0.100 inch) or more into the material, the durometer is 0 for that scale. If it does not penetrate at all, then the durometer is 100 for that scale. It is for this reason that multiple scales exist. Durometer is a dimensionless quantity, and there is no simple relationship between a material's durometer in one scale, and its durometer in any other scale, or by any other hardness test.
Durometers of various common materials Material Durometer Scale Bicycle gel seat 15-30 OO Chewing gum 20 OO Sorbothane 40 OO Sorbothane 30-70 A Rubber band 25 A Door seal 55 A Automotive tire tread 70 A Soft wheels of rollerskates and skateboard 78 A Hydraulic O-ring 70-90 A Hard wheels of rollerskates and skateboard 98 A Ebonite Rubber 100 A Solid truck tires 50 D Hard hat (typically HDPE) 75 D
Relation between Shore hardness and elastic modulus
where E is the Young's modulus in MPa and S is the Shore hardness. This relation gives a value of at S = 100 but departs from experimental data for S < 40.
Another relation that fits the experimental data slightly better is
where erf is the error function and E is in units of Pa.
A first order estimate of the relation between Shore D hardness and the elastic modulus for a conical indenter with a 15 degree cone is 
where SD is the Shore-D hardness and E is in MPa.
Another linear relation between the Shore hardness and the logarithm of Young's modulus is applicable over a large range of Shore A and Shore D hardnesses. This relation has the form:
where SA is the Shore A hardness, SD is the Shore D hardness, and E is the Young's modulus in MPa.
- US patent 1770045, A.F. Shore, "Apparatus for Measuring the Hardness of Materials", issued 1930-07-08
- US patent 2421449, J.G. Zuber, "Hardness Measuring Instrument", issued 1947-06-03
- Brinell hardness test
- Bloom (test)
- Knoop hardness test
- Leeb Rebound Hardness Test
- Rockwell hardness test
- Vickers hardness test
- ^ a b "Shore (Durometer) Hardness Testing of Plastics". http://www.matweb.com/reference/shore-hardness.asp. Retrieved 2006-07-22.
- ^ "Material Hardness". CALCE and the University of Maryland. 2001. http://www.calce.umd.edu/general/Facilities/Hardness_ad_.htm#3.5. Retrieved 2006-07-22.
- ^ a b "Rubber Hardness". National Physical Laboratory, UK. 2006. http://www.npl.co.uk/server.php?show=ConWebDoc.379. Retrieved 2006-07-22.
- ^ a b "DuroMatters! Basic Durometer Testing Information". CCSi, Inc.. http://www.ccsi-inc.com/t-durometer-testing.pdf. Retrieved 29 May 2011.
- ^ A.N. Gent, (1958), On the relation between indentation hardness and Young's modulus, Institution of Rubber Industry -- Transactions, 34 , pp. 46–57.
- ^ British Standard 903, (1950,1957), Methods of testing vulcanised rubber Part 19 (1950) and Part A7 (1957).
- ^ a b Qi, HJ and Joyce, K. and Boyce, MC, (2003), Durometer hardness and the stress-strain behavior of elastomeric materials, Rubber Chemistry and Technology, 76(2), pp. 419-435.
Wikimedia Foundation. 2010.
Look at other dictionaries:
Shore (disambiguation) — A shore is the fringe of land at the edge of a large body of water.Shore may also refer to: *Shoring, supporting a structure in order to prevent collapse so that construction can proceed *Shore durometer, the hardness of a material *Jersey Shore … Wikipedia
Shore hardness — a hardness measure determined by a Shore durometer. See duro … Dictionary of units of measurement
Skateboard — Skateboarder in the air A … Wikipedia
Barcol hardness test — The Barcol hardness test characterizes the indentation hardness of materials through the depth of penetration of an indentor, loaded on a material sample and compared to the penetration in a reference material. The method is most often used for… … Wikipedia
Rockwell scale — The Rockwell scale is a hardness scale based on the indentation hardness of a material. The Rockwell test determines the hardness by measuring the depth of penetration of an indenter under a large load compared to the penetration made by a… … Wikipedia
Inline speed skating — is the sport of racing on inline skates. It is often called inline racing by participants. Although it primarily evolved from racing on quad roller skates, the sport is similar enough to ice speed skating that many competitors are now known to… … Wikipedia
Tygon Tubing — Tygon is a brand name for a variety of flexible tubing. Tygon is a registered trademark of Saint Gobain Corporation. It is an invented word, owned and used by Saint Gobain and originated in the late 1930s. Tygon is produced in 3 countries but… … Wikipedia
international rubber hardness degree — (IRHD) a unit used to measure the hardness of rubber and similar materials (technically known as elastomers). Measurements are made using an IRHD durometer, and the results are usually similar, but not identical, to readings made with the… … Dictionary of units of measurement
Radial shaft seal — Radial shaft seals are used to seal rotary elements, such as a shaft or rotating bore. Common examples include strut seals, hydraulic pumps seals, axle seals, power steering seals, and valve stem seals. Early radial shaft seals utilized rawhide… … Wikipedia
Твёрдость по Шору (Метод вдавливания) — У этого термина существует и другое значение, см. Твёрдость по Шору. При этом следует понимать, что хотя в другом значении этот метод также является методом измерения твёрдости, оба метода предложены одним и тем же автором, имеют совпадающие… … Википедия